2. § INTRODUCTION
§ THERMAL COMFORT
§ HEAT BALANCE
§ HEAT LOSS
§ AIR PERMEABILITY
§ EFFECT ON FABRIC PROPERTIES
§ MOISTURE TRANSPORT
§ SENSORIAL COMFORT
§ WATER ABSORPTION
§ WATER REPELLENCY
3. COMFORT !!...TEXTILE PROPERTY..? NO
Is Your clothing comfortable?
What are some of the factors that influence your answer with regard to the
clothes that you are presently wearing ?
It is likely that some of the tactile characteristics of fabrics like fabric
hand, drape, stiffness, will influence your answer.
It may also depend on how the garment fit or even on psychological
factors, such as how you feel or weather you like the garments that you are
Other factors that may influence your answer are weather you feel hot,
cold, dry, or damp wearing these particular garments.
4. Factors having to do with heat, moisture, and air are associated with thermal
comfort, which has been defined as “ that condition of mind which expresses
satisfaction with the thermal environment.”
Comfort is both physiological and psychological. It is not a textile property; it
is a human feeling, a condition of ease or well being that is influenced by many factors
including textile properties.
Previous part of the Unit was focused on tactile properties of textiles, some of
which influence comfort as well as aesthetics.
This part focuses on the physical properties of the textile materials that can
influence the thermal comfort of the wearer or user of textile items.
5. A significant factor in physical comfort has to do with temperature and
moisture. Weather the wearer is comfortable wearing a garment made of a particular
textile fabrics depends, in part, on the properties of the fabrics that either promote or
restrict the passage of heat, air or moisture vapor through the fabrics.
Clothing contributes to the temperature regulating system of the body.
Heat and moisture transfer are fairly well defined in physical terms; however,
the subjective component of comfort is equally or more important.
This part of Unit addresses physical factors that can relate to comfort
including: heat, moisture, and air; textile tests for assessing the transfer of heat,
moisture, and air through fabrics, and the related structural properties of textiles.
6. In case of clothing, apparel fabrics provide a boundary between
the micro-environment immediately surrounding the body and the
larger indoor or outdoor environment. In the case of interior
furnishing fabrics, such as draperies, blankets, or carpets, textile
form the boundary between two larger environments. In either
case, weather the fabric takes on the role of barrier or transporter
depends on the physical characteristics of the textile.
The points to consider in Thermal Comfort are…
Measurement of thermal conductivity
Measurement of water vapour permeability
7. HEAT BALANCE
The human body tries to maintain a constant core temperature of
The actual value varies slightly from person to person but the
temperature of any one person is maintained within narrow limits.
In most climates body temperature is above that of the external
environment so that there has to be an internal source of heat in order to
maintain the temperature difference.
The required heat comes from the body's metabolism, that is the
necessary burning of calories to provide power to the muscles and other
However, the body must be kept in thermal balance: the metabolic
heat generated together with the heat received from external sources
must be matched by the loss from the body of an equivalent amount of
If the heat gain and the heat loss are not in balance then the body
temperature will either rise or fall, leading to a serious threat to life.
8. The efficiency of the human organism is such that of the energy
taken in as food only 15-30% is converted into useful work with the
remaining 70-85 % of the energy being wasted as heat.
Any level of physical activity above that needed to maintain body
temperature will result in an excess of heat energy which must be
dissipated, otherwise the body temperature will rise.
A lower level of physical activity will lead to a fall in body temperature
if the available heat is not conserved by increased insulation.
If a person is comfortable (that is, in
heat balance) at rest then a burst of
hard exercise will mean that there is a
large amount of excess heat and also
perspiration to be dissipated. On the
other hand if the person is in heat
balance during strenuous exercise
then he or she will feel cold when
resting owing to the large reduction of
9. HEAT LOSS
There are four mechanisms that allow the body to lose heat to the
environment in order to maintain its thermal balance. The way the heat
loss is divided between the mechanisms depends on the external
10. 1 Conduction. In this process heat loss is accomplished through direct
contact with another substance. The rate of exchange is determined by
the temperature difference between the two substances and by their
thermal conductivities. For example the body loses heat in this manner
when submerged in cold water.
2 Convection. This is a process in which heat is transferred by a moving
fluid (liquid or gas). For example, air in contact with the body is heated by
conduction and is then carried away from the body by convection.
3 Radiation. This is the process of heat transfer by way of
electromagnetic waves. The waves can pass through air without
imparting much heat to it. Heat radiation and absorption by an object are
both influenced by its colour. Black is both the best absorber and radiator
4 Evaporation. Changing liquid water into vapour requires large amounts
of heat energy. If the water is evaporated from the skin surface then the
energy required is removed from the skin, thus cooling it. This
mechanism works well in a hot dry environment but evaporation of sweat
becomes a problem in hot humid climates.
11. The requirements for heat balance vary with the climate; in hot
climates the problem is one of heat dissipation whereas in cold climates it
is one of heat conservation.
Clothing has a large part to play in the maintenance of heat
balance as it modifies the heat loss from the skin surface and at the same
time has the secondary effect of altering the moisture loss from the skin.
However, no one clothing system is suitable for all occasions: a clothing
system that is suitable for one climate is usually completely unsuitable for
The main fabric properties that are of importance for maintaining
thermal comfort are:
o• Wind proofing
o• Moisture vapour permeability
These properties are closely interrelated in that changes in one
property can cause changes to the other three properties.
An air temperature of 28-290C would be required for a person to be
able to sit in comfort without wearing any clothes.
 At air temperatures lower than this, therefore, the body will lose heat
without the added insulation given by clothing.
 If losses by convection can be prevented, the air itself offers a very
high resistance to heat conduction having a value of thermal resistance
which is only slightly less than that of a vacuum.
 This heated air is then immediately replaced with cooler air either
through natural convection or through air currents.
Convection losses can therefore be reduced by keeping the air
surrounding the body at rest.
 Air tends to 'cling' to solid surfaces so that material with a large
exposed surface area, such as a mass of fine fibres, acts as a good
restrictor of air movement.
 In clothing the majority of the bulk is composed of air, for example a
worsted suiting fabric is made up of 25% fibre and 75% air whereas
knitted underwear may contain 10% or less actual fibre, with the rest
consisting of air.
13. The heat flow through a fabric is due to a combination of
conduction and radiation the convection within a fabric being negligible.
The conduction loss is determined by the thickness of the fabric and
its thermal conductivity. The thermal conductivity is itself a combination of
the conductivity of air kA and that of the fibre kF :
Fabric conductivity k = (1— f) kA + f kF
where f is the fraction by volume of the fabric taken up by fibre.
The heat flow due to radiation is more complex as it is governed by
the temperature difference between the heat emitter and the heat
absorber. The infra-red radiation only travels a few millimeters into a fabric
as it is either scattered or absorbed by the fibres. These fibres in turn emit
radiation which travels a further short distance to the next fibres and so on
until it reaches the far surface. Therefore the radioactive heat transfer
between the body and the external environment is indirect and depends on
the absorption and emission properties of the fibres.
14. In order to predict the heat flow due to radiation through a fabric it is
necessary to know the temperature profile. The simplest assumption is a
linear change in temperature with distance through the fabric which is true
of conduction heat flow. At the edges of a fabric the situation is more
complex than this, but in the centre of a thick specimen the conductivity
due to radiation can be simplified to :
σ = Stefan-Boltzmann constant (5.67 X 10-8W/m2K4),
ε = thermal emissivity,
R = radius of fibres,
T = mean temperature between heat source and sink (K),
f = fractional fibre volume.
This means that the heat loss from radiation is higher at low fibre volumes
(less than 5%) but is reduced by the use of fine fibres and higher fibre
15. The insulation value of clothing when it is worn is not just dependent on
the insulation value of each individual garment but on the whole outfit as
the air gaps between the layers of clothing can add considerably to the
total insulation value. This assumes that the gaps are not so large that air
movement can take place within them, leading to heat loss by convection.
The insulation value of a fabric is in fact mainly dependent on its
thickness and it can be estimated from the relationship:
clo = 1.6 X thickness in cm
where clo is a measure of thermal resistance
The insulation value of clothing is generally measured by its
thermal resistance which is the reciprocal of thermal conductivity. The
advantage of using thermal resistance rather than conductivity is that the
values of the different layers of clothing can then be added together to
give the overall resistance value of the outfit. The thickness of the
material is not taken into consideration in the units of thermal resistance
used. The SI unit of thermal resistance is degrees Kelvin square meter
per watt (1 unit = 1 Km2/W).
16. Two different units are in use in the clothing field:
This is an American unit which was adopted for the simplicity of
presentation to a layperson. Clothing having a thermal resistance of one
clo unit approximates the normal indoor clothing worn by sedentary
workers, i.e. suit, shirt and underwear.
The complete definition is the insulation required to maintain a
resting man producing heat at 50Kcal/m2/h indefinitely comfortable in an
atmosphere at 210C less than 50% RH and air movement of l0cm/s. Its
value is equivalent to 0.155 0Cm2/w.
This is a British unit which was proposed by workers at the Shirley
Institute and it is related to the international units for thermal resistance
used for building materials but converted to larger units to make them
easier to use:
1 tog = 0.10Cm2/W l clo = 1.55 tog
10 togs = I Km2/W = I0Cm2/W
♫ Air tends to cling to surfaces and thus form an insulating layer.
♫ This is the reason that the comfort temperature for the
unclothed body is lower than the skin temperature.
♫ However, the air layer is easily disturbed by air movements;
Fig. shows the fall in its insulation value with increasing wind
speed which is governed by the following equation : where V = air
18. Wind has two other major effects on clothing:
♣ it causes compression of the underlying fabrics and therefore reduces
their insulation value by reducing their thickness.
♣ it disturbs the trapped air in the clothing system by both the movement
of the fabric and by penetration through the fabric, thus increasing the
convection heat losses.
At low windspeeds (less than 8km/h) these effects are negligible
but at windspeeds of 32- 48km/h they can become significant depending
on the air permeability of the outer layer of the clothing. For example an
impermeable cover fabric worn over a pile insulating layer showed an
18% loss in insulation at a windspeed of 48km/h due to compression.
With the use of permeable outer fabrics the convection losses were:
10% 4.5 oz (125 g) downproof sateen
43% 5.5 oz (155g) cotton gabardine
73% 3 oz (85 g) poplin shirting
A fabric can easily be made windproof by coating it with an
impermeable coating or by using a tight weave. However, coated fabrics
have low rate of moisture vapour transmission.
19. Moisture vapour permeability
Perspiration is an important mechanism which the body uses to
lose heat when its temperature starts to rise. Heat is taken from the body
in order to supply the latent heat needed to evaporate the moisture from
There are two forms of perspiration:
1 Insensible - in this form the perspiration is transported as a vapour and it
passes through the air gaps between yarns in a fabric.
2 Liquid – in this form occurs at higher sweating rates and it wets the
clothing which is in contact with the skin.
The two forms of perspiration raise separate problems: one is the ability of water vapour to
pass through the fabric, particularly the outer layer; and the other is the ability of the fabric in
contact with the skin of absorbing or otherwise dealing with the liquid sweat.
20. ♦The ability of a fabric to allow perspiration in its vapour form to pass
through it is measured by its moisture vapour permeability in grams of
water vapour per square meter per 24 hours.
♦ A fabric of low moisture vapour permeability is unable to pass sufficient
perspiration and this leads to sweat accumulation in the clothing and
♦ The overall moisture vapour permeability of clothing is rather like the
thermal insulation value in that it depends on the whole clothing system.
The resistance of each clothing item together with air gaps adds to the
total resistance of the system.
♦ If the production of perspiration is greater than the amount the clothing
system will allow to escape, moisture will accumulate at some point in the
clothing system. If the outer layer is the most impermeable, moisture will
accumulate in the inner layers.
♦ The level of perspiration production is very dependent on the level of
activity: clothing that may be comfortable at low levels of activity may be
unable to pass sufficient moisture vapour during vigorous activity
21. Waterproof Breathable Fabrics
The existence of the problem of the lack of water vapour permeability in
waterproof fabrics has led to the development of waterproof breathable
Ω One approach to producing such a fabric is to use membranes
attached to the fabric or coatings on the fabric which are waterproof but
which will allow moisture vapour to pass through.
It is possible to achieve this
because of the enormous difference
in size between a water droplet and
a water vapour molecule. A water
droplet has a size of around 100µm
whereas a water vapour molecule
has a size of around 0.0004µm. If,
therefore, a membrane or fabric can
be produced with pore sizes
between these two limits it will then
have the desired properties.
22. Ω Another approach is to use a coating or membrane made from a
hydrophilic film without any pores. The moisture is absorbed by the
membrane and then transported across it by diffusion, evaporating when
it reaches the outer surface. The driving force for the diffusion is provided
by the body temperature which ensures that the water passes out even
when it is raining.
23. ΩA third approach is to use a tightly
woven fabric. One of the original
waterproof breathable fabrics, Ventile,
was produced in this way by using tightly
woven special cotton yarns which
swelled when wet thus closing any gaps
in the fabric. The production of fine
microfibres has allowed the production of
fabrics that are woven sufficiently tightly
to keep liquid water out.
Waterproofing is very important for the outer layer of a clothing
system designed to be worn outdoors. This property is particularly
important in cold weather activities for keeping the insulation of any
clothing system dry. Waterlogging of fabrics fills up the air spaces with
water and hence reduces their insulation value considerably. If the water
penetrates to the skin it can also remove a large amount of heat by the
same mechanism as that which makes perspiration effective.
The waterproofing of fabrics can readily be achieved by the use
of synthetic polymer coatings; however, the use of simple coatings bring
with it the penalty of excess build-up of moisture vapour above certain
levels of activity. The design of clothing for comfort and protection in
adverse weather conditions is therefore a matter of compromise between
the competing requirements. No one fabric or clothing item can fulfill all
the requirements, the clothing system as a whole has to be considered.
25. AIR PEARMEABILITY
The air permeability of a fabric is a measure of how well it allows
the passage of air through it. The ease or otherwise of passage of air is of
importance for a number of fabric end uses such as industrial filters,
tents, sailcloths, parachutes, raincoat materials, shirtings, downproof
fabrics and airbags.
† AIR PERMEABILITY The air permeability of a fabric is the
volume of air measured in cubic centimeters passed per second
through 1cm2 of the fabric at a pressure of 1cm of water.
† AIR RESISTANCE The air resistance of a fabric is the time in
seconds for 1cm3 of a air to pass through 1cm2 of the fabric
under a pressure head of 1cm of water.
† AIR POROSITY The porosity of a fabric is a ratio of airspace to
the total volume of the fabric expressed as a percentage.
26. MEASUREMENT OF AIR PERMEABILITY
The Shirely air permeability
apparatus is illustrated in fig. 7.12.
Air at 20 ± 2OC and 65 ± 2 % R.H.
is drawn from the laboratory
through the test specimen S by
means of a suction pump A, the
rate of flow being controlled by
means of the by pass valve B and
the series valve C.
The rate of flow is adjusted until the required pressure drop across the
fabric is indicated on a draught gauge D, graduated from 0 to 25mm
water head. For fabrics of high resistance, the rate of flow of air through
the specimen is inadequate for proper operation of the suction pump;
this is over come by opening the by-pass valve B. Fine control is
obtained by adjusting valve C. E is reservoir which smoothes out any
disturbance due to the varying velocities of the streams of air drawn
through the various paths by the pump.
27. When the required pressure drop,
which is normally 1cm of water, is
attained and the indicator of the
draught gauge is steady, the rate of
flow of air is read off one of the four
Rotameter R, selected according to
the permeability of the test specimen
The rotameters are calibrated, at
20OC and 760 mm of mercury, to
indicate air flow in cm3 /s.
Rotameter cover the following range : R1 0.05 - 0.5 , R2 0.5 - 3.5,
R3 3 - 35 and R4 30 - 350.
Five circular specimens are clamped in the holder each with a test
area of 508mm2 (25.4mm diameter) and the mean air flow per second is
calculated from the five results and by dividing by 5.07 we obtain the air
permeability of the fabric in Cubic Centimeters per Seconds at 1 cm head of
water. Alternatively, 5.07 may be divided by mean flow; this gives air
resistance of the fabric in seconds per cubic centimeters per square
centimeter under a pressure of 1 cm of water.
28. EFFECT ON FABRIC PROPERTIES
Permeability and Cloth Cover :-
One would expect that the more open structure of the fabric the
greater the air permeability, but this relationship is not always simple
one. For example, using given yarns the ends and picks per inch may
be varied and the air permeability found to follow the variation in cloth
cover more or less as expected. However, it is possible to arrange a
series of fabrics built from yarns of different counts with the yarn
spacing adjusted to give each fabric the same cover and to find large
differences in their air permeability.
Yarn Twist is also important in that as twist increases, the
circularity and density of the yarn increases in a fabric. This reduces
the yarn diameter and the fabric cover which increases the air
Yarn crimp and weave influences the shape and area of the
interstices between the yarns and may permit yarns to extend easily.
Such yarn extension would open up the fabric, increase the free area
and increases the air permeability. Hot calendaring can be used to
flatten yarns which reduces air permeability.
THERMAL WATER VAPOUR
 Tog meter  Cup Method
 Guarded Hotplate  Sweating Guarded
Method Hotplate Method
30. MEASUREMENT OF THERMAL CONDUCTIVITY
 Practical methods of test for thermal conductivity measure the total
heat transmitted by both mechanisms i.e. by conduction through the
fibre and the entrapped air and by radiation.
 The insulation value of a fabric is measured by its thermal resistance
which is the reciprocal of thermal conductivity (transmittance) and it is
defined as the ratio of the temperature difference between the two
faces of the fabric to the rate of flow of heat per unit area normal to the
 It is necessary to know the rate of heat flow through a fabric to
measure its thermal resistance. In practice it is difficult as a heater
dissipates its heat in all directions.
 Two different methods are in use to overcome this problem:
to compare thermal resistance of the sample with that of a
known standard and
to eliminate any loss in heat other than that which passes
through the fabric being tested.
31. TOG METER
The togmeter avoids the problem of measuring heat flow by
placing a material of known thermal resistance in series
with the material under test so that the heat flow is the
same through both materials. The thermal resistance of the
test fabric can then be calculated by comparing the
temperature drop across it with the temperature drop
across the standard material.
The togmeter consists of a thermostatically controlled
heating plate which is covered with a layer of insulating board of
known thermal resistance. The temperature is measured at both
faces of this standard. The heater is adjusted so that the
temperature of the upper face of the standard is at skin
temperature (31-350C). A small airflow is maintained over the
apparatus. There are two methods of test that can be used with
32. 1 Two plate method. In this
method the specimen under test
is placed between the heated
lower plate and an insulated top
plate as shown in Fig. The top
plate has a low mass so that it
does not compress the fabric.
The temperature is measured at
the heater (T1), between the
standard and the test fabric (T2)
and between the fabric and the
top plate (T3).
33. 2 Single plate method. In this
method the specimen under test
is placed on the heated lower
plate as above but it is left
uncovered as shown in Fig., the
top plate being used to measure
the air temperature (T3). The air
above the test specimen has a
considerable thermal resistance
itself so that the method is in fact
measuring the sum of the
34. To determine the air resistance : The heater and the fan
are switched on and the apparatus is allowed to reach thermal
equilibrium with no specimen present. The top plate is placed
underneath the apparatus shielded from radiation by a foil-covered plate,
in order to measure the air temperature. The temperature should remain
steady at each thermocouple for 30 mins. It may take some time for an
equilibrium to be reached. Thermal resistance of air:
To determine the sample resistance : The above
experiment is repeated with the test sample placed on the bottom plate
and the apparatus again allowed to reach thermal equilibrium. Thermal
resistance of sample:
35. GUARDED HOT PLATE
The guarded hotplate is used to
measure thermal transmittance
which is the reciprocal of the
thermal resistance. The apparatus
consists of a heated test plate
surrounded by a guard ring and with
a bottom plate underneath as
shown in Fig.
With the test fabric in place the apparatus is allowed to reach
equilibrium before any readings are taken. This may take some time with
thick specimens. The amount of heat passing through the sample in
watts per square meter is measured from the power consumption of the
test plate heater. The temperature of the test plate and the air 500mm
above the test plate are measured.
36. All three plates consist of heating
elements sandwiched between
aluminum sheets. All the plates
are maintained at the same
constant temperature in the range
of human skin temperature (33-
360C). The guard ring and bottom
plate, which are maintained at the
same temperature as the test
plate, ensure that no heat is lost
apart from that which passes
upwards through the fabric under
test. The whole apparatus is
covered by a hood to give still air
conditions around the specimen.
The whole of the surroundings of
the apparatus is maintained at
fixed conditions between 4.5 and
21.10C and 20 and 80% RH, the
exact conditions being specified
as part of the test.
37. The measured thermal transmittance consists of the thermal
transmittance of the fabric plus the thermal transmittance of the air layer
above the fabric which is not negligible. Therefore the test is repeated
without any fabric sample present to give the bare plate transmittance.
The transmittance of the air layer above the plate is assumed to be the
same as that of the air layer above the sample.
The bare plate transmittance Ubp is similarly
calculated and then the intrinsic transmittance
of the fabric alone, U2, is calculated from the
38. Measurement of water vapour permeability
ö The water vapour permeability of fabrics is an important property for
those used in clothing systems intended to be worn during vigorous
ö The human body cools itself by sweat production and evaporation
during periods of high activity. The clothing must be able to remove this
moisture in order to maintain comfort. This is an important factor in cold
ö The main materials of interest are those fabrics that incorporate a
polymer layer that makes the fabric waterproof but which still allows some
water vapour to pass through.
ö There are two main types of these materials:
those that contain pores through which the moisture vapour can
those containing a continuous layer of hydrophilic polymer.
39. ö The mechanism of water vapour transmission through the second type
is quite different from that of the first type.
ö In particular the rate of diffusion through the hydrophilic polymer layer is
dependent on the concentration of water vapour in the layer. The higher
the concentration, the higher the rate of transfer.
ö In the materials where transmission is via pores the rate is independent
of water vapour concentration.
ö This has a bearing on the results obtained from the different methods of
testing water vapour permeability.
40. CUP METHOD
In the British Standard version of this method the specimen under
test is sealed over the open mouth of a dish containing water and placed
in the standard testing atmosphere. After a period of time to establish
equilibrium, successive weightings of the dish are made and the rate of
water vapour transfer through the specimen is calculated.
The water vapour permeability index is calculated by expressing
the water vapour permeability (WVP) of the fabric as a percentage of the
WVP of a reference fabric which is tested alongside the test specimen.
41. Each dish is filled with sufficient distilled water to give a 10mm air gap
between the water surface and the fabric. A wire sample support is placed
on each dish to keep the fabric level. Contact adhesive is applied to the
rim of the dish and the specimen, which is 96mm in diameter, is carefully
placed on top with its outside surface uppermost. The cover ring is then
placed over the dish and the gap between cover ring and dish sealed with
PVC tape as shown in Fig.
A dish which is covered with the reference fabric is also set up in
the same way. All the dishes are then placed in the standard atmosphere
and allowed to stand for at least 1 hr to establish equilibrium. Each dish is
then weighed to the nearest 0.001 g and the time noted. After a suitable
time for example overnight the dishes are reweighed and the time noted
42. where WVPf is the water vapour permeability of the test fabric and
WVPr is the water vapour permeability of the reference fabric.
The experiment is sometimes carried out with the cup
inverted so that the water is in contact with the inner surface of the
fabric [U]. This form of the test tends to give more favorable results
for hydrophilic films
43. Sweating guarded hotplate method
It is similar to the guarded hotplate which is used to measure
thermal resistance. If the plate is saturated with water the power required
is then related to the rate at which water evaporates from the surface of
the plate and diffuses through the material in addition to the dry thermal
In order to measure the water vapour permeability of a material,
therefore, it is first necessary to measure the dry thermal transmittance
U1. The measurement is then repeated with the plate supplied with
moisture. This is achieved by using a saturated porous plate covered with
a Cellophane film, as shown in Fig., which allows moisture to pass
through but not in sufficient quantity to wick into the fabric.
44. A moisture vapour permeability index im is calculated from the following
45. In order to keep the wearer dry and hence comfortable,
clothing that is worn during vigorous activity, such as sports
clothing, has to be able to deal with the perspiration produced by
There are two main properties of clothing, that affect the
handling of moisture.
Firstly there is the ease with which clothing allows the
perspiration to be evaporated from the skin surface during the
Secondly after the activity has ceased, there is a need for
the moisture that is contained in the clothing layer next to the skin
to dry out quickly.
This ensures that the wearer does not lose heat
unnecessarily through having a wet skin.
46. Moisture is transmitted through fabrics in two ways:
1 By diffusion of water vapour through the fabric. This appears to be
independent of fibre type but is governed by the fabric structure.
2 By the wicking of liquid water away from the skin using the mechanism
of capillary transport. The ability of a fabric to do this is dependent on the
surface properties of the constituent fibres and their total surface area.
The size and number of the capillary paths through the fabric are also
very important. Also the rate of wicking may be different along the warp
(wale) direction than along the weft (course) direction.
The points to consider in Moisture transport are…
Ю For wicking to take place the fibre has first to be wet by the liquid.
Ю In fact it is the balance of forces involved in wetting the fibre surface
that drives the wicking process.
Ю When a fibre is wetted by a liquid the existing fibre-air interface is
displaced by a new fibre-liquid interface.
Ю The forces involved in the equilibrium that exists when a liquid is in
contact with a solid and a vapour at the same time are given by the
48. The contact angle is defined as the angle between the solid surface and
the tangent to the water surface as it approaches the solid; the angle is
shown as θ in Fig. The angle is determined by the three interfacial
tensions: if γSV is larger than γSL then cos θ is positive and the contact
angle must be between 0° and 90°. If γSV is smaller than γSL then the
contact angle must be between 90° and 180°. A high contact angle for
water with the surface means that water will run off it, a low contact
angle means that water will wet the material. A contact angle of less than
90° also means that water will wick into the material by capillary action. A
contact angle of 90° or more means that water will not rise by capillary
▲ In the absence of external forces the transport of liquids into
fibrous assemblies is driven by capillary forces that arise from the
wetting of the fibre surfaces described above.
▲ If the liquid does not wet the fibres it will not wick into the
fibrous assembly. In the case of contact angles above 90°, liquid
in a capillary is depressed below the surface instead of rising
▲ In order for the wicking process to take place spontaneously,
the balance of energy has to be such that energy is gained as the
liquid advances into the material, therefore γSV must be greater
50. The wicking rate is dependent on the capillary dimensions of the fibrous
assembly and the viscosity of the liquid. For a simple capillary of radius r
the rate of progress of the liquid front shown diagrammatically in Fig. 8.10
is given by:
The wetting of fibres is purely
dependent on their surface properties,
in particular in the case of wetting with
water, whether the surface is
hydrophobic or hydrophilic. Therefore
the wetting and wicking properties of
fibres can be modified by surface
When wicking takes place in a
material whose fibres can absorb
liquid the fibres may swell as the liquid
is taken up, so reducing the capillary
spaces between fibres, potentially
altering the rate of wicking.
51. LONGITUDINAL WICKING
52. WICKING TEST
In this test a strip of fabric is
suspended vertically with its lower
edge in a reservoir of distilled water as
shown in Fig. The rate of rise of the
leading edge of the water is then
monitored. A dye can be added to the
water or, the conductivity of the water
may be used to complete an electrical
circuit to detect the position.
The measured height of rise in a given time is taken as a direct indication
of the wickability of the test fabric. The simple form of the test does not
take into account the mass of the water that is taken up. This will depend
on the height the water has risen to, the thickness of the fabric and the
water-holding power of the fabric structure. One way of allowing for this is
to weigh the fabric at the end of the test and hence obtain the mass of the
water taken up by the fabric. The mass can then be expressed as a
percentage of the mass of the length of dry fabric which is equivalent to
the measured height of water rise.
53. TRANSVERSE WICKING
Transverse wicking is the transmission of water through the thickness of a
fabric, that is, perpendicular to the plane of the fabric.
It is perhaps of more importance than longitudinal wicking because the
mechanism of removal of liquid perspiration from the skin involves its
movement through the fabric thickness.
Transverse wicking is more difficult to measure than longitudinal wicking
as the distances involved are very small and hence the time taken to
traverse the thickness of the fabric is short.
One test is the plate test which consists of a horizontal sintered glass
plate kept moist by a water supply whose height can be adjusted so as
to keep the water level precisely at the upper surface of the plate. A
fabric placed on top of this glass plate as shown in Fig. can then draw
water from the glass plate at a rate which depends on its wicking power.
It is important that the water level is adjusted to touch the underside of
the fabric but not to flood it.
54. The rate of uptake of water is measured by timing the movement of the
meniscus along the long horizontal capillary tube. Given the diameter of
the capillary tube, the mass of water taken up by the fabric in a given time
can be calculated. A problem encountered with this method is that a load
has to be placed on top of the fabric to ensure contact with the sintered
glass plate. Unfortunately when a fabric is compressed its structural
elements are moved closer to one another which can potentially change its
absorption characteristics. A contact pressure of 0.098 kPa has been
55. Sensorial comfort is concerned with how a fabric or garment feels when it
is worn next to the skin. It has been found that when subjects wore various
fabrics next to the skin they could not detect differences in fabric structure,
drape or fabric finish but could detect differences in fabric hairiness. Some
of the separate factors contributing to sensorial comfort which have been
1 Tickle caused by fabric hairiness.
2 Prickle caused by coarse and therefore stiff fibres protruding from
3 Wet cling which is associated with sweating and is caused by damp
and sticky sweat residues on skin.
4 Warmth to touch when a garment is first picked up or put on it is usually
at a lower temperature than the skin and thus there will be a loss of
heat from the body to the garment until the temperatures of the
surfaces in contact equalise.
56. Some textile end uses such as towels, tea towels, cleaning
cloths, nappies (diapers) and incontinence pads require the material to
There are two facets to the absorption of water: one is the total
amount that can be absorbed regardless of time and the other is the
speed of uptake of the water.
These two properties are not necessarily related as fabrics of
similar structures but with different rates of uptake may ultimately hold
similar amounts of water if enough time is allowed for them to reach
The points to consider in Water Absorption are....
▼ Static Immersion
▼ Wettability of Textile Fabrics
▼ Sinking Time
57. STATIC IMMERSION
The static immersion test is a method for measuring the total
amount of water that a fabric will absorb. Sufficient time is allowed in
the test for the fabric to reach its equilibrium absorption.
Four specimens each 80mm X 80mm are cut at 45° to the warp
direction. The first step is to condition the samples and weigh them.
They are then immersed in distilled water at a temperature of 20 ± I0C
to a depth of 10cm. A wire sinker is used to hold the specimens at the
required depth. The samples are left in this position for 20min. After the
specimens are taken from the water the surface water is removed
immediately from them by shaking them ten times in a mechanical
shaker. They are then transferred directly to preweighed airtight
containers and then reweighed and weight of water absorbed is
calculated as a percentage of the dry weight of the fabric.
The mean percentage absorption is calculated.
58. Wettability of textile fabrics
This is a test for fabrics containing hydrophilic fibres. Wettability
is defined as the time in seconds for a drop of water or 50% sugar
solution to sink into the fabric. Fabrics that give times exceeding 200 sec.
are considered unwettable.
In the test the specimen is clamped onto an embroidery frame
150mm in diameter so that it is held taut and away from any surface. A
burette with a standard tip size (specified in the standard) is clamped
6mm above the horizontal surface of the sample as shown in Fig.
59. The fabric is illuminated at an angle of 45° and is viewed at 45° from the
opposite direction so that any water on the surface reflects the light to the
viewer. At the start of a test a drop of liquid is allowed to fall from the
burette and the timer started. When the diffuse reflection from the liquid
vanishes and the liquid is no longer visible, the timing is stopped. If the
time recorded is less than 2s, the burette is changed to one containing
50% sugar solution. Five areas on each specimen are tested, three
samples in all, to give a total of 15 measurements.
This is a simple test for highly absorbent materials in which a
25mm X 25mm piece of fabric or a 50mm length of yarn taken from the
fabric is dropped onto the surface of distilled water and the length of time
it takes to sink is measured. If the sample does not sink within 1 min it is
considered as having floated.
60. A number of fabric end uses, particularly those where fabric is
used out of doors, require the material to be more or less impermeable to
rain. These include outerwear such as raincoats and also industrial
fabrics such as tents and tarpaulins. Broadly two main categories of
resistance to water penetration are recognized, based mainly on the
treatment that has been used on the fabric:
1 Waterproof. A
waterproof fabric is one that is coated or impregnated to form a
continuous barrier to the passage of water using for example rubber,
polyurethane, PVC or wax coatings. In such fabrics the gaps between the
yarns are filled in by the coating which gives rise to two main drawbacks.
Firstly the fabric will no longer allow water vapour to pass through
it, making it uncomfortable to wear when sweating.
Secondly the binding together of the yarns by the coating
reduces the ability of the fabric to shear and thus to mould to the body
61. 2 Showerproof. Showerproof
fabrics are ones that have been treated in a such a way as to delay the
absorption and penetration of water. Showerproofing of fabrics is often
achieved by coating them with a thin film of a hydrophobic compound
such as a silicone. When a fabric has been treated in this way a drop of
water on the surface does not spread. The process leaves the gaps in the
fabric weave untouched so keeping it quite permeable to air and water
vapour. However, water can penetrate the fabric if it strikes it with
sufficient force as in heavy rain.
The points to consider in Water Repellency are…
× Spray Ratings
× Bundesmann Water Repellency Test
× WIRA Shower Test
× Credit Rain Simulation Tester
× Hydrostatic Head
62. SPRAY RATINGS
ά The spray rating test is one used to measure the resistance of a fabric
to surface wetting but not to penetration of water.
ά It is therefore a test which is particularly used on Showerproof
In the test three specimens
are tested, each one 180mm square.
Each specimen in turn is held taut
over a 150mm diameter embroidery
hoop which is mounted at 45° to the
horizontal. A funnel which is fitted with
a standard nozzle containing 19 holes
of a specified diameter is held 150mm
above the fabric surface as shown in
Fig. Into the funnel is poured 250ml of
distilled water at 20 0C to give a
continuous shower onto the fabric.
63. After the water spray
has finished the hoop and
specimen are removed and
tapped twice smartly against a
solid object on opposite points
of the frame, the fabric being
kept horizontal. This removes
any large drops of water. The
fabric is then assigned a spray
rating either using the written
grading shown in Table or
from photographic standards
(American Association of
Textile Chemists and Colorists
64. Bundesmann water repellency test
Θ The Bundesmann test aims to
produce the effect of a rainstorm
on a fabric in the laboratory.
Θ In the test shown in Fig. the
fabric is subjected to a shower of
water from a head fitted with a
large number of standard
Θ During the shower the back of
the fabric is rubbed by a special
mechanism which is intended to
simulate the flexing effect which
takes place when the fabric is
65. In the test four
specimens are mounted over
cups in which a spring loaded
wiper rubs the back of the cloth
while the whole cup assembly
slowly rotates. They are
subjected for 10 min to a heavy
shower whose rate has been
adjusted so as to deliver 65ml of
water per minute to each cup.
The water flow is maintained at
2O0C and between pH 6 and 8.
66. Because of the large amount of water consumed the equipment has to be
connected to the mains water supply which leads to difficulties in keeping
the water temperature constant. The shower is calculated to have a
kinetic energy 5.8 times that of a cloudburst, 90 times that for heavy rain,
480 times that for moderate rain and 21,000 times that for light rain. Two
fabric parameters are determined from the test:
1 Penetration of water through the fabric: the
water collected in the cups is measured to the
2 Absorption of water by the fabric: in order to
do this the specimen is weighed before the test
and then after the shower. To remove excess
water the fabric is shaken ten times using a
mechanical shaker and then weighed in an
67. WIRA shower test
The WIRA shower tester have certain
advantages over the Bundesmann
test. These are:
1 It is not dependent on the flow of
water through fine holes in plates or
2 It uses distilled water and the
essential parts are non-metallic so
avoiding the corrosion.
3 Provision is made for detaching and
cleaning the backing material.
Penetration is often critically
dependent on the surface properties of
the backing material.
4 The apparatus is free-standing and is
not dependent on elaborate plumbing
and electrical fittings.
68. Ξ In the test four samples each one
125mm X 250mm are tested two at
Ξ Firstly the ribbed glass backing
plates are cleaned thoroughly by the
prescribed method and dried.
Ξ The filter papers, boxes and
measuring cylinders have to be
wetted out before the test starts.
Ξ The specimens are conditioned
and then weighed and mounted face
side up stretched across the ribbed
Ξ The valves are opened
simultaneously while the stop-watch
Ξ During the test the time for the
first 10ml of water to collect in the
measuring cylinders is noted.
69. Ξ The shower should stop after about 7.5 min. After 8.5 min the interceptor
is pulled forward and the specimens removed.
Ξ These are then given ten drops on the mechanical shaker and weighed in
a previously weighed airtight container.
Ξ The water penetration is measured to the nearest 0.5 ml if under 10 ml or
to the nearest 1 mI if over 10ml.
1 the mean absorption %;
2 the mean water penetration in ml;
3 if appropriate mean time for first 10ml.
70. Credit rain simulation tester
This instrument was produced to
simulate natural rain in terms of drop
size and distribution. The test subjects
a fabric to a simulated shower and
records the time taken for the water to
penetrate to the back of the fabric. The
shower is produced by dropping water
through needles onto a mesh cone
which splits the drops to give a
distribution of drop sizes similar to
natural rain. The fabric is mounted over
a printed circuit board which is
organised so that penetration of water
completes a circuit and shows the area
where penetration has taken place. An
electronic timer is automatically started
when the first drop falls and the timing
is stopped when contact is made.
71. Hydrostatic head
◙ The hydrostatic head test is primarily intended for closely woven water
◙ The hydrostatic head supported by a fabric is a measure of the
opposition to the passage of water through the fabric.
◙ In the test, shown diagrammatically in Fig., one face of the fabric is in
contact with water which is subjected to a steadily increasing pressure
until it penetrates the fabric.
◙ The pressure at which the water penetrates the fabric is noted. The
current size of circular specimen used is 100cm2 which is clamped
between rubber gaskets .
72. ◙ The pressure of the water is monitored by a water filled manometer
which measures the pressure on the specimen in cm of water.
◙ The rate of pressure increase of the water is controlled and can be
either 10cm head of water per minute or 60cm head of water per minute.
◙ The results which are obtained at the two rates of increase are not
◙ Five specimens in total are tested and the mean pressure calculated
from the results.